Advances in Materials Physics and Chemistry, 2015, 5, 368-373 Published Online September 2015 in SciRes. http://www.scirp.org/journal/ampc http://dx.doi.org/10.4236/ampc.2015.59037
How to cite this paper: Rodrguez, C.I.R., Mancilla, J.R.F., Chavez, K.E.V., Magaa, F.E., Mndez, S.F.O. and Galindo, J.T.E. (2015) Effect of Thickness on Magnetic Dipolar and Exchange Interactions in SmCo/FeCo/SmCo Thin Films. Advances in Materials Physics and Chemistry, 5, 368-373. http://dx.doi.org/10.4236/ampc.2015.59037
Effect of Thickness on Magnetic Dipolar and Exchange Interactions in SmCo/FeCo/SmCo Thin Films Carlos Ivn Rodrguez Rodrguez1,2, Jos Rurik Faras Mancilla1, Karla Edith Vega Chavez2, Francisco Espinosa Magaa3, Sion Federico Olive Mndez3, Jos Trinidad Elizalde Galindo1 1Instituto de Ingeniera y Tecnologa, Universidad Autnoma de Ciudad Jurez, Ciudad Jurez, Mxico 2Universidad Tecnolgica de Ciudad Jurez, Ciudad Jurez, Mxico 3Centro de Investigacin de Materiales Avanzados (CIMAV), Chihuahua, Mxico Email: firstname.lastname@example.org Received 10 June 2015; accepted 1 September 2015; published 4 September 2015
Copyright 2015 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY). http://creativecommons.org/licenses/by/4.0/
SmCo/FeCo/SmCo trilayer was deposited with two different thickness configurations for soft phase (FeCo); 50 nm/10 nm/50 nm and 50 nm/25 nm/50 nm were deposited on Si (111) sub-strate and Ta (50 nm) seed layer by RF magnetron sputtering in a pressure, p, of 30 - 35 m Torr. After deposition the films were annealed under Ar atmosphere at temperature T equal to 923 and 973 for different times followed by quenching in water. X-ray diffraction patterns were obtained to identified phase presents and calculate average crystallite size. To study the effect of configura-tion thickness in soft phases, DC magnetic measurements were carried out; the measurements were done in the temperature interval of 300 - 50 K. Hysteresis loops collected at low tempera-tures exposed an increment in coercivity with the decrease of T and at same time, presented a knee in the second quadrant of the demagnetization curve, which suggests that the inter-layer exchange coupling becomes less effective, being more evident for sample with 50 nm/25 nm/50 nm thickness. Moreover, M (H) plots were calculated from magnetic measurements at three dif-ferent temperatures, T, equal to 300, 150 and 50 K, which corroborates that the dipolar interac-tions became stronger when thickness of soft phases increases. Finally, the thickness effect is at-tributed to the SmCo5 phase magnetocrystalline anisotropy constant, which is responsible for the exchange coupling length.
Keywords Exchange Interactions, Dipolar Interaction, Anisotropy
C. I. R. Rodrguez et al.
1. Introduction Kneller and Hawig  first introduce an exchange spring composite magnet consisted of hard and soft magnets. The hard magnetic phase provides a high coercive force while the soft phase offers a high magnetization. Then, Skomski and Coey  predicted a giant energy product (BH)max with theoretical value of 120 MGOe using this exchange spring. Since the magnetic properties and the degree of exchange coupling are strongly dependent on the microstructural parameters, phase distribution, volume and crystallite size. The nanocomposite multilayer films can be prepared by the technique such melt spinning -, mechanical milling -, sputtering - and nanoparticle assembly . Nanocomposite multilayer films prepared by sputtering are of the state of the art in permanent magnets and, its interest is not only for understanding the mechanism of nanocomposite magnets but also for developing the next generation of magnets .
For the last two decades, many researchers focused their research on the exchange coupling in the interface between the hard and soft phases , the temperature dependence of the exchange spring bilayers, the effect of inter-diffusion at the interface on exchange coupling and the effect of controlled composition interface on ex-change spring magnet -.
In this paper, we report the study of effect thickness in magnetic dipolar and exchange interaction in the tri-layer SmCo/FeCo/SmCo. It was found a strong dependence of soft layer thickness in the exchange and dipolar interactions at low temperature measurements.
2. Experimental SmCo/FeCo/SmCo thin films were deposited on Si (100) substrate by RF magnetron sputtering system with a base pressure of 5 106 Torr. SmCo and FeCo were deposited by SmCo target composition and FeCo target composition. A Ta underlayer and Ta cap layer also were deposited by RF magnetron sputtering Ta target (puri-ty of 99.95%). Ar pressure was kept at range of 30 - 35 m Torr. Two different thickness configurations for soft phase (FeCo): 50 nm/10 nm/50 nm and 50 nm/25 nm/50 nm were deposited; the thickness of Ta, SmCo and FeCo layer were controller by Inficon microbalance. The as-deposited film were annealed in vacuum at different temperature T equal to 923 K for 60 min and 973 K for 15 min followed by quenching in water. X-ray diffrac-tion (XRD) patterns were obtained using a Panalytical XPert MPD diffractometer with Cu-K radiation in a 2 ranging from 30 - 60 with a step size of 0.008 and time for step 30 s. Magnetic hysteresis loops were meas-ured on a Quantum Design VersaLab vibrating sample magnetometer (VSM) in fields up to 30 kOe at tempera-ture, T, ranging from 300 to 50 K.
3. Results and Discussion Figure 1 shows XRD pattern obtained for thickness variation in the soft phase from 10 to 25 nm and annealing temperature from 923 K for 60 minutes to 973 K for 30 minutes, respectively. To understand the magnetic be-havior of multilayer system just FeCo soft layer thickness changed, SmCo hard layer thickness was constant to 50 nm. In DRX SmCo and FeCo diffraction peaks are very small due the formation of most SmCo and FeCo clusters were amorphous associated with few small crystallites . All phases in samples were identified with SmCo5 (PDF2-00-027-1122), Fe65Co35 (PDF2-00-048-1817), Ta (PDF2-00-002-1104), TaO2 (PDF2-00-019- 1297), Ta2O5 (PDF2-00-018-1304). The as-deposited sample was amorphous. Therefore, it is evident that as heat treatment was carried out, the (111) peak of the SmCo5 appears and also the (110) peak of Fe65Co35.
The M-H loops of SmCo/FeCo/SmCo samples annealed at T = 923 K for 60 minutes and T = 973 K for 30 minutes were measurement by VSM with a magnetic field of 30 kOe applied in substrate plane direction. Figure 2 shows the hysteresis loops of SmCo/FeCo/SmCo films with different thickness for soft phase, annealed at dif-ferent temperature. Samples annealed at 973 K for 30 minutes and 923 K for 60 minutes were deposited with 10 and 25 nm for FeCo layer, respectively. The VSM measurement temperature was in the range between 300 and 50 K. The demagnetization curve at 300 K has a smooth convex profile that, according to Kneller and Hawig, correspond to a fully exchange coupled nanocomposite. Meanwhile, as temperature decrease, the sample with FeCo layer with 10 nm thickness exhibits a little Knee in the second quadrant and the Knee for sample with FeCo layer with 25 nm thickness is much more pronounced. This effect has been interpreted as an exchange de-coupling due to the difference in the thickness of FeCo layer  .
C. I. R. Rodrguez et al.
Figure 1. XRD of SmCo/FeCo/SmCo films with different thickness and heat treatment.
Figure 2. Hysteresis loop of SmCo/FeCo/SmCo films measured in low temperature range T = 300 - 50 K.
Figure 3 shows maximum magnetization, Mr, remanence, and Mmax, remanence to maximum magnetization ratio, Mr/Mmax, and coercivity, HC, behavior of SmCo/FeCo/SmCo films samples annealed at T = 923 K for 60 minutes and T = 973 K for 30 minutes. The measurement temperature was in the range between 300 and 50 K. For soft layer thickness of 10 nm the Mmax and Mr shows a little increment upon cooling besides HC increase by more than 400% when temperature is lowered to 50 K. This behavior can be attributed to the exchange coupling present because the hard layer. Besides, for soft layer thickness of 25 nm, Mmax and Mr shows a similar behavior but for lower temperature, 50 K, a significant decoupling between both phases, soft and hard, can be expected because the knee appearing in the second and four quadrant close to cero applied field. This behavior is attri-buted to the dipolar interaction present because the soft layer thickness. M curves were calculated to determine the behavior of thin films system when the soft layer thickness
changes. Below we describe, how these curves have the potential to yield information about the magnetic inte-ractions in two-phase magnetic nanocomposites. M plots are defined starting from the observation that an assembly of uniaxial magnetically-noninteraction
single-domain particles obeys the relationship:
C. I. R. Rodrguez et al.
( ) ( )2d m r r mM H M M H= (1) where Mr(Hm) is acquired after the application and subsequent removal of a directly applied field Hmax, and Md(Hm) is the direct current demagnetization remanence measured after applying the maximum positive mag-netic field Hmax (starting from the demagnetized state), and then applying and removing a negative m